advertisement

PHYSICAL REVIEW B 80, 104438 共2009兲 Theory of unconventional metamagnetic electron states in orbital band systems Wei-Cheng Lee and Congjun Wu Department of Physics, University of California, San Diego, California 92093, USA 共Received 7 February 2009; revised manuscript received 9 September 2009; published 30 September 2009兲 We extend the study of the Fermi surface instability of the Pomeranchuk type into systems with orbital band structures, which are common features in transition metal oxides. Band hybridization significantly shifts the spectral weight of the Landau interactions from the conventional s-wave channel to unconventional non-s-wave channels, which results in anisotropic 共nematic兲 Fermi surface distortions even with ordinary interactions in solids. The Ginzburg-Landau free energy is constructed by coupling the charge-nematic, spinnematic, and ferromagnetic order parameters together, which shows that nematic electron states can be induced by metamagnetism. The connection between this mechanism and the anisotropic metamagnetc states observed in Sr3Ru2O7 at high magnetic fields is studied in a multiband Hubbard model with the hybridized quasi-onedimensional dxz and dyz bands. DOI: 10.1103/PhysRevB.80.104438 PACS number共s兲: 75.10.⫺b, 71.10.Ay I. INTRODUCTION Pomeranchuk instabilities are a large class of Fermi surface instabilities in both density and spin channels, each of which can be further decomposed into different partial wave channels.1 This class of instabilities in the non-s-wave density channel results in uniform but anisotropic 共nematic兲 electron liquid states,2 which have recently attracted a great deal of attention in recent years.2–21 In particular, these instabilities have been studied in the context of doped Mott insulators,22 high Tc materials,3,22 and quantum Hall systems in nearly half-filled Landau levels.23,24 Experimental evidence has also been found in ultrahigh mobility twodimensional electron gases and quantum wells in large magnetic fields.25–27 Non-s-wave spin channel Pomeranchuk instabilities are unconventional magnetism in analogy to unconventional superconductivity, which have been extensively investigated.2,4,5,28–32 In Ref. 28 by Wu and Zhang, these states are classified as isotropic and anisotropic phases dubbed  and ␣ phases as the counterparts of 3He-B 共isotropic兲 and A 共anisotropic兲 phases, respectively. The  phases have circular or spherical Fermi surfaces with topologically nontrivial spin configurations in momentum space.28 In the  phase, the relative spin-orbit symmetry is broken, a concept introduced in the context of 3He-B phase, while essentially the overall rotational symmetry is not. The ␣ phases are anisotropic electron liquid crystal states with spin degree of freedom, which have been studied by many groups: the p-wave phase studied by Hirsch31,32,44 under the name of the “spin-split” state, and was also proposed by Varma et al.5,30 as a candidate for the hidden order phenomenon in the heavy fermion compound URu2Si2; the d-wave phase was studied by Oganesyan et al.2 under the name of “nematic-spinnematic” phase. Systematic studies of the ground state properties and collective excitations in both the anisotropic ␣ and isotropic  phases has been performed by Wu et al.28,29 Very recently, Chubukov and Maslov found that when approaching the ferromagnetic quantum critical point, the p-wave channel spin Pomeranchuk instability develops prior to the developing of ferromagnetic instability.33 1098-0121/2009/80共10兲/104438共6兲 Although unconventional magnetism has not been convincingly identified in experiments, a spontaneous nematic electron liquid has been observed in the ultraclean samples of the bilayer ruthenate Sr3Ru2O7,34–36 which has arouse much research interest.4,37–43 Sr3Ru2O7 is a metallic itinerant system with the tetragonal RuO2 共ab兲 planes. It is paramagnetic at zero magnetic field and develops two consecutive metamagnetic transitions in the external magnetic field B perpendicular to the ab-plane at 7.8 and 8.1 T below 1K. In the state between two metamagnetic transitions, the resistivity measurements show a strong spontaneous in-plane anisotropy 共nematic兲 along the a and b axis without noticeable lattice distortions, indicating that this effect is of electronic origin. It can be interpreted35 as a nematic state with the anisotropic distortion of the Fermi surface of the majority spin polarized by the external magnetic field, which is essentially a mixture of the d-wave Pomeranchuk instabilities in both density and spin channels. In spite of years of intensive research, most theories remain phenomenological without considering the actual orbital band structures of Sr3Ru2O7.37–39 Particularly, two key questions have not been answered satisfactorily. First, Sr3Ru2O7 is a t2g-band system, containing two quasi-onedimensional bands of dxz and dyz and one two-dimensional band of dxy. Which are responsible for the nematic behavior? Second, the nematic states require strong exchange interactions in the d-wave channel, but the usual exchange interaction from Coulomb repulsion is mostly in the s-wave channel. Microscopic theories based on the single band picture of dxy combined with the van Hove singularity have been developed.4,42,43 However, their models need a large d-wave channel exchange interaction which was introduced by hand. It is difficult to justify the microscopic origin of this interaction in terms of Coulomb interaction.4,42,43 Furthermore, these theories do not address the fact that the nematic ordering does not appear in the single layer compound Sr2RuO4, which has a similar band structure of dxy. In this paper, we provide a natural answer to these two key questions by extending the theory of Pomeranchuk instabilities into multiorbital systems. We propose that it is the hybridized quasi-one-dimensional dxz and dyz bands instead of the dxy band that are responsible for the nematic ordering 104438-1 ©2009 The American Physical Society PHYSICAL REVIEW B 80, 104438 共2009兲 WEI-CHENG LEE AND CONGJUN WU based on the following reasoning. The key difference of electronic structures between Sr3Ru2O7 and Sr2RuO4 is the bilayer splitting, which is prominent for the quasi-onedimensional bands of dxz and dyz but small for the twodimensional bands of dxy. It is natural to expect that the spontaneous nematic behavior occurs in the bands of dxz and dyz and is accompanied by an orbital ordering. Furthermore, the orbital band hybridization between them shifts a significant spectral weight of the exchange interaction into the d-wave channel, thus the nematic ordering can arise from the conventional multiband Hubbard interactions. This mechanism also applies to other strongly correlated orbital systems. This paper is organized as follows. We first present a heuristic picture to illustrate the idea how orbital hybridization enhances the Landau interaction in non-s-wave channels in Sec. II. In Sec. III, a phenomenological Ginzburg-Landau free energy is constructed to explain the two consecutive metamagnetic transitions and the nematic phase in between. In Sec. IV, we use a microscopic multiorbital Hubbard model based on the quasi-one-dimensional dxz and dyz bands to explain the appearance of the nematic state. Conclusions and outlooks are made in Sec. V. II. LANDAU INTERACTIONS MODIFIED BY ORBITAL HYBRIDIZATION In this section, we present a heuristic picture to illustrate the enhancement of the non-s-wave Landau interactions from orbital band hybridizations. For a single band system without orbital structures, the Landau interaction functions can be simply expressed at the Hartree-Fock level in the density and spin channels as 1 f s共pជ 1,pជ 2兲 = V共qជ = 0兲 − V共兩pជ 1 − pជ 2兩兲, 2 1 f a共pជ 1,pជ 2兲 = − V共兩pជ 1 − pជ 2兩兲, 2 共1兲 where V共pជ 兲 is the Fourier transform of the two-body interaction V共兩rជ1 − rជ2兩兲, say, the Coulomb interaction. The high partial wave channel components of V are usually weak, thus the condition for Pomeranchuk instabilities in high partial channels is more stringent than that of the s-wave instability of ferromagnetism. This situation is significantly changed in multiband systems with nontrivial orbital hybridization. Let us consider a simplified two-dimensional example of the hybridized bands between dxz and dyz and assume the single particle eigenstates around the Fermi surface takes the form of 兩共pជ 兲典 = eipជ ·rជ兩u共pជ 兲典 丢 Fock exchange interaction of two electrons of the same spin which are not completely indistinguishable any more. Consequentially, the exchange interaction between them acquires an extra form factor describing the inner product of their orbital configurations as − V共pជ 1 − pជ 2兲兩具u共p1兲兩u共p2兲典兩2 . The Landau interaction functions change to 1 f s共pជ 1,pជ 2兲 = V共qជ = 0兲 − 关1 + cos 2共 p1 − p2兲兴 ⫻ V共pជ 1 − pជ 2兲, 4 1 f a共pជ 1,pជ 2兲 = − 关1 + cos 2共 p1 − p2兲兴V共pជ 1 − pជ 2兲. 4 III. GINZBERG-LANDAU THEORY Equation 共4兲 above implies that a strong ferromagnetic or metamagnetic 共s wave兲 tendency also enhances the nematic ordering 共d wave兲. Before constructing the microscopic theory, we illustrate this point through a Ginzburg-Landau free energy formalism which includes the coupling among the ferromagnetic order m, the charge-nematic order nc, and spin-nematic order nsp. In the square lattice, the two different nematic channels dx2−y2 and dxy belong to nonequivalent representations. Therefore we keep only the dx2−y2 channel instability which is experimentally observed. Due to the experimentally observed anisotropy between the z axis and the ab plane, we only keep the z component of spin and spin-nematic orders. The Ginzburg-Landau free energy is constructed as 2 4 + gcn4c + gsnsp + g共m兲ncnsp , F共h兲 = F共m兲 − hm + rcn2c + rspnsp 共5兲 where F共m兲 is the magnetic order contribution to the free energy as an even function of m; h is the external magnetic field; rc ⬀ 共2 + Fs2兲 and rsp ⬀ 共2 + Fa2兲 are the mass terms of charge- and spin-nematic orders, respectively; nc,sp are defined as nc = 兺 具† 共kជ 兲共kជ 兲典f共kជ 兲, kជ , nsp = 兺 具␣† 共kជ 兲z,␣共kជ 兲典f共kជ 兲, kជ , 共2兲 where p is the azimuthal angle of pជ ; 兩u共pជ 兲典 is the Bloch wave function with the internal orbital configurations; 共 = ↑ , ↓兲 are the spin eigenstates. This orbital structure has no effects on the Hartree interaction between two electrons with opposite spins, while it significantly changes the 共4兲 Therefore even if the bare interaction V共pជ 1 − pជ 2兲 is dominated by the s-wave channel, the extra d-wave factor arising from the orbital hybridization shifts a significant weight into the d-wave channel. , 兩u共pជ 兲典 = cos p兩dxz典 + sin p兩dyz典, 共3兲 共6兲 where f共kជ 兲 is a form factor exhibiting the dx2−y2 symmetry; g共m兲 is the coupling function between nc and nsp which is an odd function of m as required by time-reversal symmetry. The experimentally observed two consecutive metamagnetic transitions can be reproduced by a suitable designed form of F共m兲 sketched in Fig. 1共a兲 where only the part with m ⬎ 0 is shown. It has two common tangent lines marked with dotted 104438-2 PHYSICAL REVIEW B 80, 104438 共2009兲 THEORY OF UNCONVENTIONAL METAMAGNETIC… must have a peak satisfying Eq. 共10兲 at m2 ⬍ m ⬍ m3 but is below the critical value elsewhere as sketched in Fig. 1共b兲. Roughly speaking, the underlying physics is that metamagnetism pushes the majority Fermi surface even closely to the van Hove singularity which finally drives the nematic ordering.4 The minority Fermi surface is pushed away from critical. In the following we will confirm this mechanism explicitly in a microscopic calculation. FIG. 1. 共a兲 The sketch of the magnetic part F共m兲 in the Ginzburg-Landau free energy. The slopes of two common tangent lines mark the magnetic fields of metamagnetic transitions. 共b兲 The dimensionless coupling function g⬘共m兲 has a peak distribution between two consecutive matamagnetic transitions. and dashed lines, which touch the curve at points of m1,2 and m3,4, respectively. In the external magnetic field h, the solution of m satisfies the equation d F共m兲 = h. dm 共7兲 Therefore, the slopes of the two common tangent lines h1,2 can be interpreted as the fields at which magnetization jumps from m1 to m2 and from m3 to m4, i.e., metamagnetic transitions occur. When h lies between these two transitions, the magnetization m evolves continuously. The development of nematic orders between the two successive metamagnetic transitions is triggered by the g共m兲 term. Although the nematic instability is enhanced by Eq. 共4兲, they are still a weaker instability compared to ferromagnetism 共metamagnetism兲. This is because the condition for Pomeranchuk instability in the d-wave channel in twodimensional 共2D兲, i.e., Fs,a 2 ⬍ −2, is more stringent that in the s-wave channel, i.e., Fa0 ⬍ −1. We assume that the chargeand spin-nematic channels are close to be critical but not yet, i.e., rc,sp are small but positive. Due to the hybridization term of g共m兲, the eigenorder parameters arise from the diagonalization of the quadratic terms of nc,sp as n+ = cos nc + sin ns , IV. MICROSCOPIC THEORY FOR THE BILAYER Sr3Ru2O7 We next make the connection to Sr3Ru2O7 by exploiting a microscopic model with dxz and dyz orbital bands. They have the bonding and antibonding bands with a large bilayer splitting at the order of their band widths. Only the bonding bands, the even combination of the bilayer orbitals, are considered because their Fermi surfaces are close to van Hove singularity which enhances interaction effects. Because of orbital hybridization, they form closed Fermi surfaces. As moving around this Fermi surface, the orbital configuration varies between dxz and dyz exhibiting a d-wave pattern, thus the mechanism illustrated in Sec. II applies. The band Hamiltonian H0 reads H0 = 兺 兵⑀xz,kជ dxzkជ dxz,kជ + ⑀yz,kជ dyz,kជ dyz,kជ + kជ 共dxz,kជ dyz,kជ † † kជ 共11兲 + H.c.兲其, with ⑀xz,kជ = − 2t储 cos kx − 2t⬜ cos ky − 4t⬘ cos kx cos ky , ⑀yz,kជ = − 2t⬜ cos kx − 2t储 cos ky − 4t⬘ cos kx cos ky , kជ = 4t⬙ cos kx cos ky . H0 = 兺 Ekជ ␥+kជ ␥+kជ + Ekជ ␥−kជ ␥−kជ , 共8兲 where tanh 2 = 2g共m兲 / 共rc − rsp兲. The corresponding eigenvalues read 1 r⫾ = 兵rc + rsp ⫾ 冑共rc − rsp兲2 + 4关g共m兲兴2其. 2 关g⬘共m兲兴2 ⬅ 关g共m兲兴2 ⬎ 1. 4rcrsp 共13兲 where 冑 1 ⫾ 2 Ekជ = 关⑀xz,kជ + ⑀yz,kជ ⫾ 共⑀xz,kជ − ⑀yz,kជ 兲2 + 4hkជ 兴 2 共14兲 and the band eigenoperators reads ␥+,kជ = cos kជ dxz,kជ + sin kជ dyz,kជ , ␥−,kជ = − sin kជ dxz,kជ + cos kជ dyz,kជ , 共10兲 In the presence of the van Hove singularity of DOS, which is a common mechanism for metamagnetism, all the parameters in the GL free energy could change significantly so that the distribution of the dimensionless coupling function g⬘共m兲 may not be smooth. For the nematic order only occurring in the regime between two metamagnetic transitions, g⬘共m兲 − † kជ 共9兲 The critical coupling for the n− channel to develop the instability is 共12兲 t储 and t⬜ are the nearest-neighbor longitudinal and transverse hopping integrals for the dxz and dyz orbitals; t⬘ and t⬙ are the next-nearest neighbor intra- and interorbital hopping, respectively. The resulting diagonalized band Hamiltonian is + † n− = − sin nc + cos ns , † 共15兲 with the hybridization angle kជ satisfying tan 2kជ = 2kជ ⑀xz,kជ − ⑀yz,kជ = − 4t⬙ cos kx cos ky . t储 − t⬜ cos kx − cos ky 共16兲 This band hybridization pattern is a lattice version of Eq. 共2兲 with only the dx2−y2 channel but not the dxy channel. We 104438-3 PHYSICAL REVIEW B 80, 104438 共2009兲 WEI-CHENG LEE AND CONGJUN WU FIG. 2. 共a兲 Dispersion of the ␥+ band for kជ = 共kx , 0兲 and 共kx , 兲. 共b兲 The DOS of the ␥⫾ bands whose peaks corresponds to the van Hove singularities at kជ = 共0 , 0兲 , 共0 , 兲 , 共 , 0兲. choose the parameter values of 共t储 , t⬜ , t⬘ , t⬙兲 = 共1.0, 0.145, 0.0, 0.3兲, and plot the density of states 共DOS兲 in Fig. 2. Two peaks in the DOS exist in both ␥⫾ bands, which correspond to the van Hove singularities at kជ = 共0 , 0兲 , 共0 , 兲 , 共 , 0兲. We take the general multiband Hubbard model that are widely used in literatures for the interactions as Hint = U 兺 再 i,a=xz,yz na↑共i兲na↓共i兲 + V 兺 nxz共i兲nyz共i兲 i 1 − J 兺 Sជ xz共i兲 · Sជ yz共i兲 − nxz共i兲nyz共i兲 4 i + ⌬兺 † † 兵dxz,↑ 共i兲dxz,↓ 共i兲dyz,↓共i兲dyz,↑共i兲 FIG. 3. m and the nematic order parameter for majority spin band 共nc↑ = 共nc + nsp兲 / 2兲 versus the external field h. The topologies of the FS of the ␥+ band in each phases are sketched in the insets, where the solid and dashed lines represent the FS of the majority and the minority spin bands. ␣ ␣ = Ekជ − − Vmm − ␣共Vcnc + Vspnsp兲cos 2k , 共20兲 where k are the hybridization angle defined in Eq. 共16兲. The self-consistent equations for the order parameters read 冎 nc = nsp = + h . c.其, i 共17兲 where na, are particle number operators in orbital a with spin ; na = na,↑ + na,↓; Sជ a are spin operators in orbital a. The U term is the intraorbital repulsion; the V term is the interorbital repulsion for the spin triplet configuration of two electrons; the J term represents the Hund’s rule physics; the ⌬ term describes the interorbital pairing hopping. In the absence of the orbital hybridization, it is not conclusive that the Hubbard model can give rise to nematic transitions because on-site interactions only contribute to the s-wave channel. We define the charge-nematic order z − Szyz, and the 2nc = nxz − nyz, the spin-nematic order nsp = Sxz z z ferromagnetic order m = Sxz + Syz. The mean-field theory in the eigenbasis of ␥⫾ reads Hmf = 兺 ជ k,␣=⫾ † 2 ␣␥␣kជ ␥␣kជ + Vmm2 + Vspnsp + Vcn2c , 共18兲 where Vm = U J + , 2 4 Vsp = U J − , 2 4 Vc = V + J U − , 4 2 † 共19兲 and the less important interband coupling terms ␥+kជ ␥−kជ are dropped. The renormalized single particle spectra become 1 兺 兵n f,+,共kជ兲 − n f,−,共kជ兲其cos 2kជ , 2N k, 1 兺 兵n f,+,共kជ兲 − n f,−,共kជ兲其cos 2kជ , 2N kជ , m= 1 兺 兵n f,+,共kជ兲 + n f,−,共kជ兲其, 2N kជ , 共21兲 where the cos 2kជ factor represents the dx2−y2 symmetry of the nematic orders of nc and nsp. We are ready to study the zero-temperature phase diagram with the Zeeman energy term as Hext = − h 兺 na,共i兲. 共22兲 a=xz,yz is tuned to reach the filling of n = 3.48 at h = 0 in the bilayer bonding bands of dxz and dyz so that the FS of the ␥+ band is very close to the van Hove singularity while that of the ␥− band is far away from the singularity. The interaction parameters are chosen as 共U , V , J , ⌬兲 = 共2.7, 2.5, 0 , 0兲, which remarkably reproduce the isotropic-nematic-isotropic phase transition as a function of h as we expect from the GinzburgLandau analysis. The magnetization m and the nematic order of the majority spin Fermi surface nc,↑ = 21 共nc + nsp兲 are depicted in Fig. 3, while that of the minority spin Fermi surface is much smaller 共not shown兲 because its Fermi surface is pushed from the van Hove singularity. As explained in Ref. 4, the first jump of m distorts the Fermi surface to touch the van Hove singularity 104438-4 PHYSICAL REVIEW B 80, 104438 共2009兲 THEORY OF UNCONVENTIONAL METAMAGNETIC… points along one of the ab axes, and the second jump restores the fourfold symmetry of Fermi surface to cover the singularity in both directions. Compared to Ref. 4, the range of h for the nematic state is significantly reduced in agreement with experiment due to inclusion of the magnetic order m self-consistently in the solution. Furthermore, the first jump of m is larger than the second one as consistent with the experiments. This feature can be understood by the asymmetric profile of the DOS at the van Hove singularity which drops faster in the higher energy side as shown in Fig. 2. After the first transition, part of the FS of the majority spin has moved beyond the van Hove singularity. This reduces the DOS at the second jump and leads to a weaker second jump where the nematic order disappears. We learned another independent work by Raghu et al.45 The same mechanism is proposed for the nematic state observed in Sr3Ru2O7 based on the quasi-one-dimensional bands. They used a more detailed band structure and further considered the spin-orbit coupling effect. We further performed the Ginzburg-Landau analysis for the competition between ferromagnetization and nematic ordering. V. CONCLUSION AND OUTLOOK In this paper, we have studied the Fermi liquid instability of the Pomeranchuk type in orbital band systems. Orbital band hybridization significantly enhances the Landau interaction functions in high partial wave channels, thus providing a mechanism for the nematic states or unconventional magnetism from conventional interactions. Consequentially, metamagnetism 共ferromagnetism兲 induces the nematic behavior even with the onsite multiband Hubbard interactions. I. I. Pomeranchuk, Sov. Phys. JETP 8, 361 共1959兲. V. Oganesyan, S. A. Kivelson, and E. Fradkin, Phys. Rev. B 64, 195109 共2001兲. 3 S. A. Kivelson, I. P. Bindloss, E. Fradkin, V. Oganesyan, J. M. Tranquada, A. Kapitulnik, and C. Howald, Rev. Mod. Phys. 75, 1201 共2003兲. 4 H. Y. Kee and Y. B. Kim, Phys. Rev. B 71, 184402 共2005兲. 5 C. M. Varma, Philos. Mag. 85, 1657 共2005兲. 6 D. G. Barci and L. E. Oxman, Phys. Rev. B 67, 205108 共2003兲. 7 D. G. Barci, M. Trobo, V. Fernandez, and L. E. Oxman, Phys. Rev. B 78, 035114 共2008兲. 8 C. J. Halboth and W. Metzner, Phys. Rev. Lett. 85, 5162 共2000兲. 9 H. Y. Kee, Phys. Rev. B 67, 073105 共2003兲. 10 M. J. Lawler, D. G. Barci, V. Fernandez, E. Fradkin, and L. E. Oxman, Phys. Rev. B 73, 085101 共2006兲. 11 J. Nilsson and A. H. Castro Neto, Phys. Rev. B 72, 195104 共2005兲. 12 J. Quintanilla and A. J. Schofield, Phys. Rev. B 74, 115126 共2006兲. 13 L. Dell’Anna and W. Metzner, Phys. Rev. B 73, 045127 共2006兲. 14 I. Khavkine, C.-H. Chung, V. Oganesyan, and H.-Y. Kee, Phys. Rev. B 70, 155110 共2004兲. 15 H. Yamase and H. Kohno, J. Phys. Soc. Jpn. 69, 332 共2000兲. This mechanism is applied to the t2g system of Sr3Ru2O7 by attributing the observed nematic behavior to the hybridized quasi-one-dimensional bands of dxz and dyz, which is the major difference between our work and Refs. 4, 42, and 43. Many open questions still need future exploration. In particular, the quick suppression of the nematic behavior with the in-plane magnetic field h储 might result from the orbital effect due to the bilayer splitting as pointed out in Ref. 42, or from the spin-orbit coupling effect. The mechanism presented in this paper is also very general. It is essentially a Berry phase effect which naturally arises from electron systems with nontrivial band structures, such as spin-orbit coupling system and graphene. It can be understood as a conventional interaction acquires a nontrivial nature after projected onto a nontrivial band structure. We further predict that the nematic ordering arises at the ferromagnetic transition in spin-orbit coupling systems as a result of the hybridization between two spin components in the band structure. For example, the in-plane ferromagnetic ordering in the quasi-2D Rashba systems and the surface states of the topological insulators induces the p-wave distortion of Fermi surfaces, which will be presented in a later publication.46 ACKNOWLEDGMENTS We thank X. Dai, J. Hirsch, Y. B. Kim and H. Y. Kee for helpful discussions. C.W. is grateful for E. Fradkin, S. A. Kivelson, and S. C. Zhang for their education on Pomeranchuk instability and encouragement on this project. This work is supported by ARO-W911NF0810291 and the Sloan Research Foundation. H. Yamase and H. Kohno, J. Phys. Soc. Jpn. 70, 2733 共2001兲. H. Yamase, V. Oganesyan, and W. Metzner, Phys. Rev. B 72, 035114 共2005兲. 18 H. Yamase, Phys. Rev. B 76, 155117 共2007兲. 19 C. Honerkamp, Phys. Rev. B 72, 115103 共2005兲. 20 P. Wolfle and A. Rosch, J. Low Temp. Phys. 147, 165 共2007兲. 21 C. A. Lamas, D. C. Cabra, and N. Grandi, Phys. Rev. B 78, 115104 共2008兲. 22 S. A. Kivelson, E. Fradkin, and V. J. Emery, Nature 共London兲 393, 550 共1998兲. 23 E. Fradkin, S. A. Kivelson, E. Manousakis, and K. Nho, Phys. Rev. Lett. 84, 1982 共2000兲. 24 E. Fradkin and S. A. Kivelson, Phys. Rev. B 59, 8065 共1999兲. 25 M. P. Lilly, K. B. Cooper, J. P. Eisenstein, L. N. Pfeiffer, and K. W. West, Phys. Rev. Lett. 82, 394 共1999兲. 26 K. B. Cooper, M. P. Lilly, J. P. Eisenstein, L. N. Pfeiffer, and K. W. West, Phys. Rev. B 65, 241313共R兲 共2002兲. 27 R. R. Du, D. C. Tsui, H. L. Stormer, L. N. Pfeiffer, K. W. Baldwin, and K. W. West, Solid State Commun. 109, 389 共1999兲. 28 C. Wu and S. C. Zhang, Phys. Rev. Lett. 93, 036403 共2004兲. 29 C. Wu, K. Sun, E. Fradkin, and S. C. Zhang, Phys. Rev. B 75, 115103 共2007兲. 30 C. M. Varma and L. Zhu, Phys. Rev. Lett. 96, 036405 共2006兲. 1 16 2 17 104438-5 PHYSICAL REVIEW B 80, 104438 共2009兲 WEI-CHENG LEE AND CONGJUN WU J. E. Hirsch, Phys. Rev. B 41, 6820 共1990兲. E. Hirsch, Phys. Rev. B 41, 6828 共1990兲. 33 A. V. Chubukov and D. L. Maslov, arXiv:0908.4433 共unpublished兲. 34 S. A. Grigera, R. S. Perry, A. J. Schofield, M. Chiao, S. R. Julian, G. G. Lonzarich, S. I. Ikeda, Y. Maeno, A. J. Mills, and A. P. Mackenzie, Science 294, 329 共2001兲. 35 S. A. Grigera, P. Gegenwart, R. A. Borzi, F. Weickert, A. J. Schofield, R. S. Perry, T. Tayama, T. Sakakibara, Y. Maeno, A. G. Green, and A. P. Mackenzie, Science 306, 1154 共2004兲. 36 R. A. Borzi, S. A. Grigera, J. Ferrell, R. S. Perry, S. J. S. Lister, S. L. Lee, D. A. Tenant, Y. Maeno, and A. P. Mackenzie, Science 315, 214 共2007兲. 37 A. M. Berridge, A. G. Green, S. A. Grigera, and B. D. Simons, Phys. Rev. Lett. 102, 136404 共2009兲. 38 A. J. Millis, A. J. Schofield, G. G. Lonzarich, and S. A. Grigera, Phys. Rev. Lett. 88, 217204 共2002兲. 39 A. G. Green, S. A. Grigera, R. A. Borzi, A. P. Mackenzie, R. S. 31 32 J. Perry, and B. D. Simons, Phys. Rev. Lett. 95, 086402 共2005兲. Tamai, M. P. Allan, J. F. Mercure, W. Meevasana, R. Dunkel, D. H. Lu, R. S. Perry, A. P. Mackenzie, D. J. Singh, Z. X. Shen, and F. Baumberger, Phys. Rev. Lett. 101, 026407 共2008兲. 41 K. Iwaya, S. Satow, T. Hanaguri, N. Shannon, Y. Yoshida, S. I. Ikeda, J. P. He, Y. Kaneko, Y. Tokura, T. Yamada, and H. Takagi, Phys. Rev. Lett. 99, 057208 共2007兲. 42 C. Puetter, H. Doh, and H. Y. Kee, Phys. Rev. B 76, 235112 共2007兲. 43 H. Yamase and A. A. Katanin, J. Phys. Soc. Jpn. 76, 073706 共2007兲. 44 H. v. Löhneysen, A. Rosch, M. Vojta, and P. Wölfle, Rev. Mod. Phys. 79, 1015 共2007兲. 45 S. Raghu, A. Paramekanti, E-.A. Kim, R. A. Borzi, S. A. Grigera, A. P. Mackenzie, and S. A. Kivelson, Phys. Rev. B 79, 214402 共2009兲. 46 W. C. Lee and C. Wu 共unpublished兲. 40 A. 104438-6